General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 8.05 - 8.1 g/cm³ Show Material materials with Density of 8.05 - 8.1 g/cm³ |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | 20.0 °C | 195 GPa Show Material materials with Elastic modulus of 195 GPa |

100.0 °C | 190 GPa Show Material materials with Elastic modulus of 190 GPa | |

200.0 °C | 185 GPa Show Material materials with Elastic modulus of 185 GPa | |

300.0 °C | 179 GPa Show Material materials with Elastic modulus of 179 GPa | |

400.0 °C | 174 GPa Show Material materials with Elastic modulus of 174 GPa | |

500.0 °C | 168 GPa Show Material materials with Elastic modulus of 168 GPa | |

600.0 °C | 161 GPa Show Material materials with Elastic modulus of 161 GPa | |

700.0 °C | 154 GPa Show Material materials with Elastic modulus of 154 GPa | |

800.0 °C | 142 GPa Show Material materials with Elastic modulus of 142 GPa | |

900.0 °C | 130 GPa Show Material materials with Elastic modulus of 130 GPa | |

1000.0 °C | 119 GPa Show Material materials with Elastic modulus of 119 GPa | |

Elongation | 20.0 °C | 30 - 35 % Show Material materials with Elongation of 30 - 35 % |

Elongation A100 | 20.0 °C | 20 - 30 % Show Material materials with Elongation A100 of 20 - 30 % |

Elongation, transverse | 20.0 °C | 30 % Show Material materials with Elongation, transverse of 30 % |

Hardness, Brinell | 20.0 °C | 190 - 210 [-] Show Material materials with Hardness, Brinell of 190 - 210 [-] |

Tensile strength | 20.0 °C | 500 - 750 MPa Show Material materials with Tensile strength of 500 - 750 MPa |

100.0 °C | 520 - 530 MPa Show Material materials with Tensile strength of 520 - 530 MPa | |

200.0 °C | 490 - 515 MPa Show Material materials with Tensile strength of 490 - 515 MPa | |

300.0 °C | 480 - 500 MPa Show Material materials with Tensile strength of 480 - 500 MPa | |

400.0 °C | 470 - 490 MPa Show Material materials with Tensile strength of 470 - 490 MPa | |

450.0 °C | 465 - 485 MPa Show Material materials with Tensile strength of 465 - 485 MPa | |

Unlock all property charts | ||

Tensile strength, transverse | 20.0 °C | 550 - 750 MPa Show Material materials with Tensile strength, transverse of 550 - 750 MPa |

Yield strength Rp0.2 | 20.0 °C | 220 - 240 MPa Show Material materials with Yield strength Rp0.2 of 220 - 240 MPa |

100.0 °C | 190 - 205 MPa Show Material materials with Yield strength Rp0.2 of 190 - 205 MPa | |

150.0 °C | 175 - 190 MPa Show Material materials with Yield strength Rp0.2 of 175 - 190 MPa | |

200.0 °C | 165 - 180 MPa Show Material materials with Yield strength Rp0.2 of 165 - 180 MPa | |

250.0 °C | 160 - 175 MPa Show Material materials with Yield strength Rp0.2 of 160 - 175 MPa | |

300.0 °C | 155 - 170 MPa Show Material materials with Yield strength Rp0.2 of 155 - 170 MPa | |

350.0 °C | 150 - 165 MPa Show Material materials with Yield strength Rp0.2 of 150 - 165 MPa | |

400.0 °C | 145 - 160 MPa Show Material materials with Yield strength Rp0.2 of 145 - 160 MPa | |

450.0 °C | 140 - 155 MPa Show Material materials with Yield strength Rp0.2 of 140 - 155 MPa | |

Unlock all property charts | ||

Yield strength Rp0.2, transverse | 20.0 °C | 220 - 235 MPa Show Material materials with Yield strength Rp0.2, transverse of 220 - 235 MPa |

Yield strength Rp1.0 | 20.0 °C | 250 - 270 MPa Show Material materials with Yield strength Rp1.0 of 250 - 270 MPa |

100.0 °C | 220 - 235 MPa Show Material materials with Yield strength Rp1.0 of 220 - 235 MPa | |

150.0 °C | 205 - 220 MPa Show Material materials with Yield strength Rp1.0 of 205 - 220 MPa | |

200.0 °C | 190 - 205 MPa Show Material materials with Yield strength Rp1.0 of 190 - 205 MPa | |

250.0 °C | 185 - 200 MPa Show Material materials with Yield strength Rp1.0 of 185 - 200 MPa | |

300.0 °C | 180 - 195 MPa Show Material materials with Yield strength Rp1.0 of 180 - 195 MPa | |

350.0 °C | 175 - 190 MPa Show Material materials with Yield strength Rp1.0 of 175 - 190 MPa | |

400.0 °C | 170 - 185 MPa Show Material materials with Yield strength Rp1.0 of 170 - 185 MPa | |

450.0 °C | 165 - 180 MPa Show Material materials with Yield strength Rp1.0 of 165 - 180 MPa | |

Unlock all property charts | ||

Yield strength Rp1.0, transverse | 20.0 °C | 250 - 265 MPa Show Material materials with Yield strength Rp1.0, transverse of 250 - 265 MPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | 100.0 °C | 1.41E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.41E-5 1/K | |

200.0 °C | 1.49E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.49E-5 1/K | ||

300.0 °C | 1.52E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.52E-5 1/K | ||

400.0 °C | 1.56E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.56E-5 1/K | ||

500.0 °C | 1.58E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.58E-5 1/K | ||

600.0 °C | 1.6E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.6E-5 1/K | ||

700.0 °C | 1.67E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.67E-5 1/K | ||

800.0 °C | 1.72E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.72E-5 1/K | ||

900.0 °C | 1.76E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.76E-5 1/K | ||

1000.0 °C | 1.79E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.79E-5 1/K | ||

Unlock all property charts | |||

Max service temperature, long | -10 - 450 °C Show Material materials with Max service temperature, long of -10 - 450 °C | ||

Melting point | 1200 - 1480 °C Show Material materials with Melting point of 1200 - 1480 °C | Typical for Nickel Chromium Iron Alloy | |

Specific heat capacity | 20.0 °C | 440 J/(kg·K) Show Material materials with Specific heat capacity of 440 J/(kg·K) | |

100.0 °C | 462 J/(kg·K) Show Material materials with Specific heat capacity of 462 J/(kg·K) | ||

200.0 °C | 488 J/(kg·K) Show Material materials with Specific heat capacity of 488 J/(kg·K) | ||

300.0 °C | 514 J/(kg·K) Show Material materials with Specific heat capacity of 514 J/(kg·K) | ||

400.0 °C | 540 J/(kg·K) Show Material materials with Specific heat capacity of 540 J/(kg·K) | ||

500.0 °C | 565 J/(kg·K) Show Material materials with Specific heat capacity of 565 J/(kg·K) | ||

600.0 °C | 590 J/(kg·K) Show Material materials with Specific heat capacity of 590 J/(kg·K) | ||

700.0 °C | 615 J/(kg·K) Show Material materials with Specific heat capacity of 615 J/(kg·K) | ||

800.0 °C | 655 J/(kg·K) Show Material materials with Specific heat capacity of 655 J/(kg·K) | ||

900.0 °C | 680 J/(kg·K) Show Material materials with Specific heat capacity of 680 J/(kg·K) | ||

1000.0 °C | 710 J/(kg·K) Show Material materials with Specific heat capacity of 710 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 10.8 W/(m·K) Show Material materials with Thermal conductivity of 10.8 W/(m·K) | |

100.0 °C | 12.4 W/(m·K) Show Material materials with Thermal conductivity of 12.4 W/(m·K) | ||

200.0 °C | 14.1 W/(m·K) Show Material materials with Thermal conductivity of 14.1 W/(m·K) | ||

300.0 °C | 15.6 W/(m·K) Show Material materials with Thermal conductivity of 15.6 W/(m·K) | ||

400.0 °C | 16.9 W/(m·K) Show Material materials with Thermal conductivity of 16.9 W/(m·K) | ||

500.0 °C | 18.3 W/(m·K) Show Material materials with Thermal conductivity of 18.3 W/(m·K) | ||

600.0 °C | 19.6 W/(m·K) Show Material materials with Thermal conductivity of 19.6 W/(m·K) | ||

700.0 °C | 21 W/(m·K) Show Material materials with Thermal conductivity of 21 W/(m·K) | ||

800.0 °C | 23.2 W/(m·K) Show Material materials with Thermal conductivity of 23.2 W/(m·K) | ||

900.0 °C | 25.7 W/(m·K) Show Material materials with Thermal conductivity of 25.7 W/(m·K) | ||

1000.0 °C | 28.1 W/(m·K) Show Material materials with Thermal conductivity of 28.1 W/(m·K) | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 1.12E-6 Ω·m Show Material materials with Electrical resistivity of 1.12E-6 Ω·m |

100.0 °C | 1.14E-6 Ω·m Show Material materials with Electrical resistivity of 1.14E-6 Ω·m | |

200.0 °C | 1.18E-6 Ω·m Show Material materials with Electrical resistivity of 1.18E-6 Ω·m | |

300.0 °C | 1.2E-6 Ω·m Show Material materials with Electrical resistivity of 1.2E-6 Ω·m | |

400.0 °C | 1.24E-6 Ω·m Show Material materials with Electrical resistivity of 1.24E-6 Ω·m | |

500.0 °C | 1.26E-6 Ω·m Show Material materials with Electrical resistivity of 1.26E-6 Ω·m | |

600.0 °C | 1.26E-6 Ω·m Show Material materials with Electrical resistivity of 1.26E-6 Ω·m | |

700.0 °C | 1.27E-6 Ω·m Show Material materials with Electrical resistivity of 1.27E-6 Ω·m | |

800.0 °C | 1.28E-6 Ω·m Show Material materials with Electrical resistivity of 1.28E-6 Ω·m | |

900.0 °C | 1.29E-6 Ω·m Show Material materials with Electrical resistivity of 1.29E-6 Ω·m | |

1000.0 °C | 1.3E-6 Ω·m Show Material materials with Electrical resistivity of 1.3E-6 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Aluminium | 0.2 % Show Material materials with Aluminium of 0.2 % |

Carbon | 0.025 % Show Material materials with Carbon of 0.025 % |

Chromium | 19.5 - 23.5 % Show Material materials with Chromium of 19.5 - 23.5 % |

Cobalt | 1 % Show Material materials with Cobalt of 1 % |

Copper | 1.5 - 3 % Show Material materials with Copper of 1.5 - 3 % |

Iron | 20.04 % Show Material materials with Iron of 20.04 % |

Manganese | 1 % Show Material materials with Manganese of 1 % |

Molybdenum | 2.5 - 3.5 % Show Material materials with Molybdenum of 2.5 - 3.5 % |

Nickel | 38 - 46 % Show Material materials with Nickel of 38 - 46 % |

Phosphorus | 0.02 % Show Material materials with Phosphorus of 0.02 % |

Silicon | 0.5 % Show Material materials with Silicon of 0.5 % |

Sulfur | 0.01 - 0.015 % Show Material materials with Sulfur of 0.01 - 0.015 % |

Titanium | 0.6 - 1.2 % Show Material materials with Titanium of 0.6 - 1.2 % |